Embed Size (px)
Electronic Supplementary Material (ESI)
Synergistic Effect of Atomically Dual-metal Doped Catalyst for
Highly Efficient Oxygen Evolution
Daobin Liua‡, Shiqing Dinga‡, Chuanqiang Wua, Wei Ganad, Changda Wanga, Dengfeng Caoa, Zia
ur Rehmana, Yuan Sanga, Shuangming Chena*, Xusheng Zhenga, Yu Wangc, Binghui Geb, Li
a National Synchrotron Radiation Laboratory, Department of chemical physics, CAS Center for
Excellence in Nanoscience, University of Science and Technology of China. Hefei, Anhui 230026,
b Beijing National Laboratory for Condensed Mater Physics, Institute of Physics, Chinese
Academy of Sciences, Beijing 100190, China
c Shanghai Synchrotron Radiation Facility, Shanghai Institute of Applied Physics, Chinese
Academy of Sciences, Shanghai 201204, China
d Institute for Frontier Materials, Deakin University, Geelong Waurn Ponds Campus, Waurn
Ponds, VIC 3216, Australia
*Corresponding author: [email protected] (S. Chen); [email protected] (L. Song)
‡ These authors contributed equally to this work.
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.This journal is © The Royal Society of Chemistry 2018
Preparation of the [email protected]/CNT catalyst.
Multi-walled carbon nanotubes (MWCNTs) (Nanjing XFNANO Materials Tech Co., Ltd)
were first purified and oxidized according to the previous report. Typically, 1g CNT was calcined
at 350 ºC for 1h in the air, and washed with dilute HCl for several times to eliminate metal
impurities. After drying, the oxidized CNT was added to 23 mL concentrated H2SO4 and stirred
for 20 h at room temperature. Then 350 mg of NaNO3 were added, followed by slow addition of 1
g of KMnO4 at 40 ℃ in a water bath. The mixture was stirred for 30 min and 3 mL of water were
added, followed by another 3 mL of water after 5 min. After another 5 min, 40 mL of water were
added, followed by stirring for 15 min. The solution was removed from water bath and 140 mL of
water and 10 mL of 30% H2O2 were added. Finally, the mildly oxidized CNT were collected,
washed repeatedly with diluted HCl and water and dried it.
250 mg dicyandiamide (DCDA) was dissolved in 32 mL deionized water, and then added 4
mL NiCl2 6H2O (0.0125 M) and 4 mL FeCl3 6H2O (0.0125 M) solution. Then it was stirred at 80
℃ for 3 h. After cooling to the room temperature, 1.25 g NH4Cl and 120 mg the oxidized CNT
was added into the solution, combined with sonication to get homogeneous dispersion, and
followed by lyophilization to dry it. The obtained powder was treated at 550 ºC with a ramp rate
of 2.3 ºC min-1 for 4h in N2 atmosphere (denoted as [email protected]/CNT). For comparison,
preparation of the single-metal doped catalyst ([email protected]/CNT and [email protected]/CNT) and the
hybrid without NH4Cl ([email protected]/CNT_w/o NH4Cl) were the same as [email protected]/CNT,
except the raw materials were without the addition of FeCl3 6H2O, NiCl2 6H2O and NH4Cl,
respectively. Note that the amounts of metal precursors in these hybrids were consistent with that
of [email protected]/CNT. The g-C3N4/CNT hybrid was prepared using DCDA, MWCNTs and
NH4Cl as precursors without metal salts.
Transmission electron microscopy (TEM) and high-resolution TEM images were collected
on a JEM-2100F field emission electron microscope at an accelerating voltage of 200 kV.
Aberration-corrected high-angle annular dark-field scanning transmission electron microscopy
(HAADF-STEM) measurements and energy dispersive X-ray spectra (EDS)-mapping images,
using a 200 kV JEM-ARM200F equipped with double spherical aberration correctors. Field
emission scanning electron microscopy (FESEM) images were taken on a JEOL JSM-6700F SEM.
The PerkinElmer Optima 7300 DV ICP-AES instrument was used to determine the metal loading
content after digesting the as-obtained sample in HNO3. X-ray diffraction (PXRD) patterns were
obtained using a Japan Rigaku DMax-γA rotation anode X-ray diffractometer equipped with
graphite monochromatized Cu Kα radiation (λ = 1.54178 Å). X-ray photoelectron spectroscopy
(XPS) spectra was measured on a Thermal Fisher ESCALAB250Xi spectrometer equipped with
an Al anode (Al Kα= 1486.7 eV). The N2 adsorption-desorption experiments were carried out
using Micromeritics ASAP 2020 instrument. XAFS spectra were collected at MCD endsation in
the National Synchrotron Radiation Laboratory (NSRL), the beamline 14W1 in Shanghai
Synchrotron Radiation Facility (SSRF) and the beamline 1W1B in the Beijing Synchrotron
Radiation Facility (BSRF).The acquired EXAFS data were fit using the FEFF8.2 code.
Typically, 5 mg of catalyst was first dispersed in 1 mL solution (water/isoproparol = 1:1, v/v)
and sonicated to obtain a homogeneous ink, followed by the addition of 50 μL 5 wt.% Nafion
solution (the amount of binder has little influence on the catalyst conductivity and the intrinsic
OER performance). A certain amount of the ink was deposited on the polished glassy carbon
electrode (different diameter of glassy carbon disk in rotating disk electrode (RDE) (5.0 mm) and
rotating ring-disk electrode (RRDE) (5.61 mm), normalized to the loading area with 0.382 mg cm-
2) and dried at room temperature. All electrochemical measurements were performed on the
CHI760E (CH Instruments, China) electrochemical workstation with a standard three-electrode
setup. A graphite rod and saturated Ag/AgCl served as the counter and reference electrodes,
respectively. All potentials were calibrated to the reversible hydrogen electrode (ERHE = EAg/AgCl +
1.025 V), and all polarization curves were without iR compensation.
RDE measurements were performed in O2-saturated 1 M KOH electrolyte from 1 to 1.8 V (vs.
RHE) with a speed of 1600 rpm and a scan rate of 5 mV s-1. Electrochemical impedance
spectroscopy (EIS) measurements were carried out at an overpotential of η=350 mV, from 105 to
0.1 Hz, with an AC amplitude of 5 mV. Cyclic voltammetry were conducted between 0.925 and
1.125 V (vs. RHE) from 5 to 100 mV s-1 in order to investigate the electrochemical active surface
area (ECSA) of catalysts. The stability of [email protected]/CNT was evaluated using 3,000
continuous cycles from 1.2 to 1.6 V (vs. RHE) in O2-saturated 1M KOH at a scan rate of 100 mV
s-1, and the chronopotentiometry method at the current density of 10 mA cm-2 for 18h. Note that
the catalyst was loaded onto carbon paper with the area of 1 cm2 (Toray, TGP-H-60) for stability
To detect the production of H2O2, the rotating ring-disk electrode (RRDE) measurements
were conducted in N2-saturated 1 M KOH electrolyte from 1 to 1.8 V (vs. RHE) with a speed of
1600 rpm and a scan rate of 5 mV s-1, and the Pt-ring electrode potential was set to 1.4 V (vs.
RHE). The Faradaic efficiency was calculated by the equation of Iring/(NIdisk) (where Iring and Idisk
are the current response of Pt-ring and disk electrode, respectively, and N is the collection
efficiency of the RRDE which was determined to be ~0.37), and the corresponding experiments
were performed under the same conditions, except that the disk current was maintained at 480 μA
and the Pt-ring electrode potential was set to 0.5 V (vs. RHE) to reduce the formation of O2.
Fig. S1 (a) and (c) FESEM images, (b) and (d) TEM images of [email protected]/CNT and [email protected]
C3N4/CNT_w/o NH4Cl, respectively.
Fig. S2 Nitrogen adsorption-desorption isotherm of [email protected]/CNT, [email protected]/CNT_w/o
NH4Cl and g-C3N4/CNT.
Fig. S3 XRD patterns of [email protected]/CNT, g-C3N4/CNT, CNT and C3N4, where showed no
additional peaks corresponding metal nanoparticles.
Fig. S4 HAADF-STEM images of [email protected]/CNT in different region, indicating that Ni/Fe
atoms were anchored on g-C3N4/CNT supports without any aggregations.
Fig. S5 Wavelet transform (WT) Ni K-edge EXAFS spectra of (a) [email protected]/CNT, (b) Ni foil
and (c) NiPc. And WT Fe K-edge EXAFS spectra of (d) [email protected]/CNT, (e) Fe foil and (f)
Fig. S6 The corresponding R space fitting curve of NiFe@ g-C3N4/CNT at Ni K-edge (a) and Fe K-edge (b).
Fig. S7 The XPS survey (a), C 1s (b) and N 1s (c) high-resolution spectra of NiFe@ g-C3N4/CNT.
Fig. S8 Typical polarization curves of as-prepared hybrids with different ratio of DCDA/CNT (a) and Ni/Fe species (b).
The result in Fig. S8a reveals that the OER activity was enhanced with the increase of CNT content but dramatically decreased in [email protected]/CNT160, because of the relatively low proportion of active [email protected]. It confirmed that CNT skeletons play an important role of conductive additive to accelerate the electron transfer in catalytic process. Fig. S8b clearly shows that the trend of apparent OER activity resembles the “volcano curve” by altering the Ni/Fe ration in as-prepared hybrids. The [email protected]/CNT hybrid has a better OER activity compared to that of other hybrids. The catalytic performance was delayed with an excessive Fe species, resulting from the relatively low Ni sites in high oxidation states.
Fig. S9 CVs of NiFe@ g-C3N4/CNT (a) and [email protected]/CNT_w/o NH4Cl (b) measured in non-Faradaic region at different scan rate. (c) The current difference was calculated at 1.125 V (vs. RHE) as a function of scan rate. (d) Specific activity of [email protected]/CNT and [email protected]/CNT w/o NH4Cl was normalized by ECSA.
Fig. S10 The detection of H2O2 production by RRDE measurement (Ering= 1.40 V).
Table S1 Ni K-edge structural parameters of [email protected]/CNT and the reference NiPc and Fe
foil materials extracted from quantitative EXAFS fitting curves (σ2 is Debye-Waller factor).
N (coordination number)
Bond length σ2(10-3 Å2)
Ni-N1 3.2 1.86 6.9
Ni-O 1.0 2.08 7.3
Ni-Ni 0.6 2.49 9.2Ni-N1 4 1.89 4.8Ni-O 2 2.12 6.5Ni-C 8 2.76 11.1
Ni-N2 4 3.18 7.8Ni foil Ni-Ni 8 2.48 6.2
Note: Ni-N1 and Ni-N2 showing in the table represents the nearest and the next nearest Ni-N
Table S2 Fe K-edge structural parameters of [email protected]/CNT and the reference NiPc and Fe
foil materials extracted from quantitative EXAFS fitting curves (σ2 is Debye-Waller factor).
Bond length σ2(10-3 Å2)
Fe-N1 3.5 1.96 5.1Fe-O 1.2 2.05 3.6Fe-C 4.1 2.87 3.3
Fe-Fe 0.3 2.89 9.7Fe-N1 4 2.01 4.8Fe-O 2 2.04 3.2Fe-C 8 3.01 1.6
Fe-N2 4 3.39 9.9Fe-Fe 8 2.46 5.0Fe foil
Fe-Fe 6 2.83 5.0
Note: Fe-N1 and Fe-N2 showing in the table represents the nearest and the next nearest Fe-N
Table S3 Comparison of OER performance in alkaline with other metal-free catalysts and carbon-
based catalysts coupled with metal-Nx structure.
CatalystTafel slope(mV dec-1)
η@10 mA cm-2 (mV)
CNNTS 383 450 0.1 M KOH [S1]Co4N/CNW/CC 81 330 1 M KOH [S2]
Co/N-CNTs 67 390 0.1 M KOH [S3]S,N-Fe/N/C-CNT 82 370 0.1 M KOH [S4]
OCC-8 82 492 0.1 M KOH [S5]Co-C3N4/CNT 68.4 380 0.1 M KOH [S6]
N-GRW 47 360 1 M KOH [S7]g-C3N4 and CNTs 83 350 0.1 M KOH [S8]
N/C -- 380 0.1 M KOH [S9]
[email protected]/CNT 67 326 1 M KOH This work
Reference1. R. M. Yadav, J. Wu, R. Kochandra, L. Ma, C. S. Tiwary, L. Ge, G. Ye, R. Vajtai, J. Lou and P. M. Ajayan, ACS. Appl. Mater. Inter., 2015, 7, 11991-12000.2. F. Meng, H. Zhong, D. Bao, J. Yan and X. Zhang, J. Am. Chem. Soc., 2016, 138, 10226-10231.3. Y. Liu, H. Jiang, Y. Zhu, X. Yang and C. Li, J. Mater. Chem. A, 2016, 4, 1694-1701.4. P. Chen, T. Zhou, L. Xing, K. Xu, Y. Tong, H. Xie, L. Zhang, W. Yan, W. Chu, C. Wu and Y. Xie, Angew. Chem. Int. Ed., 2017, 56, 610-614.5. N. Cheng, Q. Liu, J. Tian, Y. Xue, A. M. Asiri, H. Jiang, Y. He and X. Sun, Chem. Commun., 2015, 51, 1616-1619.6. Y. Zheng, Y. Jiao, Y. Zhu, Q. Cai, A. Vasileff, L. H. Li, Y. Han, Y. Chen and S. Z. Qiao, J. Am. Chem. Soc., 2017, 139, 3336-3339.7. H. B. Yang, J. Miao, S. F. Hung, J. Chen, H. B. Tao, X. Wang, L. Zhang, R. Chen, J. Gao, H. M. Chen, L. Dai and B. Liu, Sci. Adv., 2016, 2, e1501122.8. T. Y. Ma, S. Dai, M. Jaroniec, S. Z. Qiao, Angew. Chem. Int. Ed., 2014, 53, 7281-7285.9. Y. Zhao, R. Nakamura, K. Kamiya, S. Nakanishi and K. Hashimoto, Nat. Commun., 2013, 4, 2390.